HIGH TEMPERATURE CORROSION INHIBITION PERFORMANCE OF IMIDAZOLINE AND AMIDE
Huey J. Chen
Chevron Petroleum Technology Company
P.O. Box 6045, L3064
San Ramon, CA 94583-0745
Tao Hong and W. Paul Jepson
NSF I/UCRC Corrosion and Multiphase Technology Center
Russ College of Engineering & Technology
Athens, OH 45601-2979
Imidazoline and its precursor, amide, are very effective inhibitor intermediates and are widely used in formulating
the corrosion products for application in the oil and gas industries. Their high temperature corrosion inhibition performance
was evaluated and compared. Our results show that imidazoline and amide offer poor to moderate high temperature/pressure
(300 °F/3,000 psig) inhibition performance, respectively, with amide giving a better thermos stability. Yet, both give
excellent, comparable inhibition performance at a moderate temperature of 150 °F. These chemistries can provide up to 90%
effectiveness at the high temperature, if the inhibitor concentration is very high.
Keywords: Corrosion Inhibitor, Inhibition, Imidazoline, Amide, High Temperature/Pressure, Performance Evaluation.
The application of corrosion inhibitors to a producing oil or gas field system is one of the most common means of
corrosion control. Corrosion inhibitors used in the oil producing industry are, in general, formulated with the following
ingredients: active inhibitor intermediate(s), carboxylic acid or dimer-trimer acid, demulsifier and/or surfactant in aromatic
solvent, and alcohol.
The inhibitor intermediate is the active component contributing to corrosion protection in the formulation. Almost all
active inhibitor intermediates used in the oil and gas industry are nitrogen-containing compounds. These compounds are
excellent inhibitors because of the free pair electrons in nitrogen atoms that can be adsorbed on a metal surface and their
hydrocarbon chain to form hydrophobic film on the surface, thus providing inhibition. 15 Different inhibitor intermediates
can often be manufactured from the same raw materials by varying the reacting conditions such as temperature or raw
materials ratios. Because raw materials used in the reaction are generally low cost and not pure, the resultant inhibitor
intermediates are, therefore, not high purity products and are oftentimes a mixture of reaction products.
©2000 by NACE International.Requests for permission to publish this manuscript in any form, in part or in whole must be in writing to NACE
International, Conferences Division, P.O. Box 218340, Houston, Texas 77218-8340. -Ihe material presented and the views expressed in this
paper are solely those of the author(s) and are not necessarily endorsed by the Association. Printed in U.S.A.
Although there are many active inhibitor intermediates on the market, they are based on a few generic types of
chemistries, namely, imidazoline, amide, amidoamide and amine. When these compounds are formulated into commercial
products, their inhibition performance varies depending on how the products are put together, but not by a significant
degree as long as the chemistry o f the intermediate is similar. These amine-based corrosion inhibitors are known not to
have high temperature inhibition performance with the upper limit temperature of about 300°°F, yet no such data is
available in the literature.
It is in our interest to develop high performance corrosion inhibitors for high temperature and high shear flow
application. A high performance corrosion inhibitor which improves performance and film life at high temperature and
high shear will increase reliability of corrosion inhibition and less reliance on expensive corrosion resistant alloy thus
reducing capex as well as opex. In order to establish the baseline data for current commercial products, we conducted a
high temperature performance evaluation for the most effective inhibitor intermediates, namely, imidazoline and amide.
Amide is a precursor of imidazoline during the manufacturing process and the conversion process from amide to
imidazoline is not a chemical reaction that can be easily controlled to obtain 100% conversion to imidazoline. The degree
of conversion varies among vendors. Amide is a solid wax while imidazoline is a viscous, free flow compound which
makes it easier for formulating a corrosion product in comparison to amide. Thus, the imidazoline intermediate used for
product formulation is, in fact, a mixture of imidazoline and the amide and their ratio can vary from 1 : 1 (50% conversion)
to 9:1 (90% conversion) depending on the manufacture's process.
Separation of amide and imidazoline is not an easy task and is unnecessary because amide is also an excellent
corrosion inhibitor. Amide is also a hydrolyzed product of imidazoline under normal operating conditions. 67 The fact that
imidazoline is a mixture may be more beneficial to overall inhibition by providing a synergistic inhibition effect.
Therefore, establishing the inhibition performance of amide is very desirable. If the amide performs as well as that of
imidazoline, the effect of amide on the performance of the resultant imidazoline will be minimal and the quality control for
manufacturing imidazoline intermediate will be less of a concern.
The objective for this investigation was to obtain the baseline performance data at high temperature/pressure for an
imidazoline and its precursor amide through the conventional weight loss method. This paper summarizes and compares
the inhibition performance of imidazoline and amide at high temperature and high pressure (300 °F and 3,000 psi), together
with performance testing under normal conditions of 150 °F. A commercial tall oil imidazoline, which is a reaction product
of tall oil fatty acid and diethylenetriamine at 1:1 mole ratio, and its precursor amide were obtained from a chemical
Inhibitor Intermediates Evaluated. Two inhibitor intermediates used in this study were obtained from a chemical
vendor through private communication. They are designated as HJC_I3238, an imidazoline and its amide precursor, HJC-
A196. They are the reaction product of tall oil fatty acid and diethylenetriamine at 1:1 mole ratio and the percent conversion
from amide to imidazoline is about 65% according to the vendor. This suggests that HJC_13238, an imidazoline, in fact,
contains 35% amide, namely HJC_A196. The molecular structures of imidazoline and amide are shown below:
X_./ Imidazoline (HJC_I-3238)
R-~-NHCH2CH2NHCH2CH2NH2 Amide (HJC_A 196)
Characteristics of lmidazol ine and Amide. Amide is generally a waxy solid and is less dispersible than the
corresponding imidazoline, lmidazoline is a free flow, viscous liquid and is easier to handle in formulating products. In fact,
this is one reason that the chemical reaction is carried out at a higher temperature to produce imidazoline by chemical
vendors. For chemical vendors, blending products from solids is more difficult and costly than blending from liquids. Note
that imidazoline can be hydrolyzed to the corresponding amide under the proper conditions as reported in the literature. 67
This can be noted on many imidazoline-based products which show amide precipitate after long standing in storage.
Since no attempt is carried out by the manufacturer to separate the imidazoline and amide, key questions regarding
quality control of manufacturing these intermediates are: (1)How important is the degree of conversion from amide to
imidazoline on the performance of the resultant product, (2)Is imidazoline more effective than amide or vice versa. If the
inhibition performance of amide and imidazoline are comparable, the quality control of imidazoline manufacturing will become
less a concern. For inhibition performance, recent literature s reported that amide gave better inhibition performance than
irnidazoline. That report showed that it requires smaller amide inhibitor concentration to give a constant corrosion rate of 2 mpy.
There are very few literaUare reports on the direct comparison of performance between amide and imidazoline. The performance
of these chemicals at high temperature is not available.
Formulat ions for Inhibition Testing. To facilitate the performance evaluation, these two inhibitor intermediates
are formulated with acetic acid in isopropyl alcohol and water at 25% active as shown in Table 1. HJC-A is formulated with
25% imidazoline, HJC_I3238, and HJC-B is formulated with 25% amide, HJC A196. A 25% active inhibitor concentration
is comparable to that of the commercial products. Thus, the inhibitor concentration tested based on these formulations will
be comparable to that of the concentration used in the commercial corrosion inhibitor product.
Inhibitor Performance Evaluation
The evaluation of the inhibitor performance at high temperature (300 °F) and high pressure (3,000 psig) conditions
was conducted at a commercial testing lab in Houston, Texas. In order to have a direct comparison of the high temperature
results, inhibitor performance at a lower temperature of 150 °F was also conducted using the conventional wheel test. Two
formulated products, HJC-A and B were evaluated according to the test conditions described below. For high temperature
and high pressure testing, inhibitors were tested at higher concentrations, namely, 100, 400, 1,000 PPM of the formulated
samples as opposed to 10, 25, and 100 PPM used in the conventional wheel test. Since the commercial products are
formulated with the active inhibitor concentration between 15-30% act